Upcoming SlideShare
×

# Polymer physics

497 views

Published on

Published in: Technology, Education
1 Like
Statistics
Notes
• Full Name
Comment goes here.

Are you sure you want to Yes No
• Be the first to comment

Views
Total views
497
On SlideShare
0
From Embeds
0
Number of Embeds
1
Actions
Shares
0
0
0
Likes
1
Embeds 0
No embeds

No notes for slide

### Polymer physics

1. 1. Chapter 5 Scaling Analysis of Polymer Dynamics 5.1 Simple Fluids In this part, we start with the basic laws of molecular motions in simple ﬂuids, to learn the scaling analysis of polymer dynamics, followed with polymer deformation and polymer ﬂow. The trajectories of Brownian motions of hard spherical molecules can be analogous to random walks. As we have leant in Chap. 2, the mean square end-to-end distance of a random walk is proportional to the number of steps, i.e. <R2 > ~ n. The three- dimensional mean-square displacement of particles in Brownian motions is also proportional to the motion time t, as <½rðtÞ À rð0Þ2 > ¼ 6 Dt (5.1) where D is the diffusion coefﬁcient. The discovery of such a law in the Brownian motion of the molecular particles is actually one of Einstein’s milestone contributions in 1905 (Einstein 1905). Accordingly, the characteristic time is deﬁned as the moving time of a particle through a distance of its own size, as t R2 D (5.2) In simple ﬂuids, the external driving forces on a small particle are equilibrated with the friction due to the collisions with its surrounding medium. Therefore, the total frictional force f is proportional to the activated constant velocity v of the moving particle with respect to its surrounding medium, as f ¼ zv (5.3) where z is the friction coefﬁcient. This law of ﬂuid dynamics is similar to the Newton’s second law for the external force proportional to the acceleration. W. Hu, Polymer Physics, DOI 10.1007/978-3-7091-0670-9_5, # Springer-Verlag Wien 2013 77
2. 2. According to the ﬂuctuation-dissipation theorem in Brownian motions (Nyquist 1928), both the driving forces and the frictional forces on a particle are initiated by the collisions of the surrounding particles with the thermal energy kT. Accordingly, we have the Einstein relationship (Einstein 1905) kT ¼ Dz (5.4) On the other hand, the frictional forces are induced by the viscosity of ﬂuids. The Stokes law reveals the relationship between the friction coefﬁcient z and the viscosity (Stokes 1851), as given by z ¼ 6pR (5.5) Therefore, one can obtain the Stokes-Einstein relationship as D ¼ kT 6pR (5.6) One can measure the viscosity and the diffusion coefﬁcient to determine the so-called hydrodynamic radius as Rh kT 6pD (5.7) This quantity of sizes reﬂects the effective volume-exclusion range of the moving particle interacting with its surrounding particles. For a single polymer chain in a good solvent, the theoretical hydrodynamic radius Rh theo can be deﬁned as 1 Rtheo h 1 n2 X i6¼j 1 rij (5.8) where . . . is an ensemble average, and n is the number of monomers in the polymer (Des Cloizeaux and Jannink 1990). Such a theoretical deﬁnition makes the hydrodynamic radius close to the radius of gyration of the polymer coil. However, as we have introduced for polymer solutions in the previous chapter, the hydro- dynamic radius of an anisotropic coil could be larger than its static radius of gyration. Thus from the dynamics point of view, the actual critical overlap concen- tration appears smaller than the theoretical prediction. In dilute solutions of hard spheres, Einstein has found that the viscosity ¼ sð1 þ 2:5cÞ (5.9) where s is the solvent viscosity, and c is the volume fraction of hard spheres (Einstein 1911). 78 5 Scaling Analysis of Polymer Dynamics
3. 3. We can regard the motion of polymer coils in a dilute solution as in the non- draining mode of spherical particles, which means that a polymer coil moves together with the holding solvent molecules, as shown in Fig. 5.1a. There is no relative velocity for those holding solvent molecules to the polymer, and all the frictional interactions for polymer motions only occur at the surface of the spherical particle. We then have c ¼ Vp V ¼ c cint \$ cR3 n (5.10) where Vp is the volume of polymer coil, V is the total volume, c is the average volume concentration of monomers, Cint is the volume concentration of monomers inside each coil, Cint ~ n/R3 , and n is the number of monomers in each chain. We deﬁne the speciﬁc viscosity sp À s s (5.11) and further deﬁne the intrinsic viscosity ½ sp c c!0j (5.12) According to (5.9), we obtain the Fox-Flory equation (Fox and Flory 1948) ½ \$ R3 n (5.13) According to the Fox-Flory equation, in a theta solvent, we can have R \$ n1=2 (5.14) from which we can further obtain the Einstein-Kuhn viscosity equation (Kuhn 1934) ½ \$ n1=2 (5.15) Fig. 5.1 Illustration of the ﬂow proﬁles for the solvent to pass through the polymer coil with (a) the non-draining mode and (b) the free-draining mode 5.1 Simple Fluids 79
4. 4. In a good solvent, R \$ n3=5 (5.16) and we can obtain the Kirkwood-Riseman equation (Kirkwood and Riseman 1948) ½ \$ n4=5 (5.17) Staudinger and Notzu considered the free-draining mode (Staudinger and Nodzu 1930), as shown in Fig. 5.1b. In this mode, the relative motion of each monomer incurs the frictional force from its surrounding solvents, which is also quite applicable to the situation of rigid polymer chains. Accordingly, ½ \$ n (5.18) A general equation summarizing all the cases above is known as Mark-Houwink equation ½ ¼ KMa (5.19) where a ranges from 0.5 to 1. From this equation, one can deﬁne the viscosity- average molecular weight, as introduced in Sect. 2.4.2 (Mark 1938; Houwink 1940). 5.2 Short Chains The characteristic feature for the motions of chain-like molecules is that, the Brownian motion of the whole chain is integrated by the Brownian motion of all the monomers. Since the motion of each monomer is restrained by the chain connection of other monomers, the Brownian motion of the polymer as a whole is slower than the small monomer molecules under comparable conditions. In other words, the diffusion coefﬁcient of polymers strongly depends on the chain length. In 1953, Rouse proposed that the ideal chain without volume exclusion (i.e. in the free-draining mode) could be treated as a coarse-grained bead-spring chain, as shown in Fig. 5.2 (Rouse 1953). Each spring connecting two beads represents a sub- molecule along the ideal chain. Its elasticity can be described by the Gaussian distribution of the distances between two ends of sub-molecules. Therefore, the total free energy contributed by the entropic elasticity is given by Eel ¼ SEi;iþ1 \$ Sðriþ1 À riÞ2 ðriþ1 À riÞ2 (5.20) 80 5 Scaling Analysis of Polymer Dynamics
5. 5. For each bead in the middle of the chain, the total elastic force results from the springs of its two sides, as given by fi ¼ À @Eel @ri \$ ðriþ1 À riÞ À ðri À riÀ1Þ ¼ @2 ri @i2 (5.21) In the case of simple ﬂuids, the force above generates a constant velocity of the bead, as given by fi ¼ z @ri @t (5.22) Therefore, we obtain the so-called Rouse equation in the continuous limit, @ri @t \$ @2 ri @i2 (5.23) Under the boundary conditions of @ri=@ij0 ¼ @ri=@ijn ¼ 0, the analytical solution of the equation above is in eigenmodes, as given by ripðtÞ ¼ ap cosð ppi n Þ expðÀ t tp Þ (5.24) where the mode number p ¼ 1, 2, 3. . . and n. n is the total number of beads on the chain and is proportional to the total amount of monomers (for the sake of simplicity in the following scaling analysis, we will directly treat n as the number of monomers). Equation (5.24) represents any term in Fourier series expansion, provided that the random-coil conformation of polymers is equally parted into p wave-lengths of a stochastic vibration holding amplitude ap. The relaxation time tp is the characteristic time for each sub-molecule to contain n/p monomers and to diffuse through its end-to-end distance Rp. Accordingly, tp \$ R2 p Dp (5.25) For an ideal chain, R2 p \$ nb2 p (5.26) Fig. 5.2 An illustration of the bead-spring model of the Rouse chain 5.2 Short Chains 81
6. 6. We know the Einstein relationship Dp ¼ kT zp (5.27) and consider the free-draining mode, zp ¼ zn p (5.28) We substitute the three equations above into (5.25), and obtain tp \$ ð n p Þ2 (5.29) When p ¼ 1, the characteristic time for each chain diffusing through its coil size is often referred as the Rouse relaxation time, i.e. tR \$ n2 (5.30) Therefore, the diffusion coefﬁcient for the whole Rouse chain is D \$ R2 1 tR \$ nÀ1 (5.31) which can also be derived directly from (5.27) and (5.28). By deﬁnition, the mean-square displacement of monomers in the time period of tp is comparable to the mean-square end-to-end distances of sub-molecules (see (5.2)). From (5.29), we have ½rðtpÞ À rð0Þ2 \$ R2 p \$ nb2 p \$ t1=2 p (5.32) Therefore, within the time window between the monomer characteristic time t0 and the whole-chain characteristic time tR, there exists following scaling relationship. ½rðtÞ À rð0Þ2 \$ t1=2 (5.33) Such a smaller scaling exponent (1/2) compared with the simple ﬂuids (1) can be attributed to the fact that the motions of monomers are slowed down due to their chain connection. Below or above this time window, the monomers or the whole chain exhibit the characteristics of simple ﬂuids, following the scaling law ½rðtÞ À rð0Þ2 \$ t (5.34) 82 5 Scaling Analysis of Polymer Dynamics
7. 7. as illustrated in Fig. 5.3. Both experiments and computer simulations on short polymer chains in the melt phase have veriﬁed such a scaling relationship of the Rouse chain. Since polymer chains in the melt are in a highly interpenetrating state, the volume exclusion effect between chain units has been well screened, and at the meantime the hydrodynamic interactions have been screened as well. Thus, the free-draining mode considered in the Rouse model is roughly applicable in the melt of short polymer chains. In dilute solutions, however, the hydrodynamic interactions could not be screened. In 1956, Zimm considered further the non- draining mode for the dynamics of single chains in dilute solutions on the basis of the Rouse model (Zimm 1956). He started with the deﬁnition of the characteristic time t ¼ R2 /D, and inserted it into the Einstein relation D ¼ kT/z. For the non- draining mode, the friction coefﬁcient of the single coil follows the Stocks law (5.5). Then he obtained tZ \$ R3 (5.35) In a good solvent, the expanded coil sizes of single chains are R ¼ bn3/5 , then the Zimm relaxation time is tZ \$ n9=5 (5.36) The scaling exponent (9/5) appears smaller than that (2) for the characteristic relaxation time of the Rouse chain. This implies that the Zimm chain diffuses faster than the Rouse chain, because the non-draining mode of the single coil incurs less frictional hindrance than the free-draining mode. Accordingly, the diffusion coefﬁcient of the Zimm chain is DZ \$ R2 tZ \$ nÀ3=5 (5.37) Similar to the derivation of the scaling law of the Rouse chain, the mean-square displacement of monomers within the time period of the characteristic time tpZ for p-mode sub-molecules is Log10[r(t)-r(0)]2 Log10t 1 1/2 1 τ0 τR nb2 b2 Rouse chain Fig. 5.3 Double logarithmic plot of the mean-square displacement of monomers versus the time, illustrating the scaling laws of the Rouse chain. Monomers are moving slower than simple ﬂuids due to their chain connection 5.2 Short Chains 83
8. 8. ½rðtpÞ À rð0Þ2 Z \$ R2 pZ \$ t 2=3 pZ (5.38) Thus we can obtain that, in the time window of t0 t tZ, corresponding to the size scale n6/5 b2 within the single coil, ½rðtÞ À rð0Þ2 Z \$ t2=3 (5.39) The exponent here (2/3) is slightly larger than that of the Rouse chain (1/2), implying again a faster diffusion. This scaling law can well describe the diffusion of a single polymer in dilute solutions. In concentrated solutions, with the increase of the polymer concentration, the screen effect of hydrodynamic interactions is enhanced due to the interpenetration of polymer chains. We can assume that the hydrodynamic screening length xh is close to the screening length of volume exclusion of monomers x, as given by xh % x (5.40) Employing the blob model for semi-dilute solutions, we deﬁne the size of the blob as x \$ g3=5 \$ CÀ3=4 (5.41) The monomers inside each blob move in a range smaller than xh, where the conditions for the non-draining mode are maintained. Therefore, the Zimm model is applicable. tx \$ x3 \$ CÀ9=4 (5.42) In contrast, beyond each blob, the motion range of monomers is larger than xh, where the conditions for the free-draining mode are restored due to the interpene- tration of polymer chains. Therefore, the Rouse model is applicable. tR \$ txð n g Þ2 \$ n2 C1=4 (5.43) The size of the blob ranges from the size of monomers to the whole chain, depending upon polymer concentrations. Therefore, the dynamic scaling law for the single short chain in the semi-dilute solutions is to insert tx between t0 and tR. In other words, the 2/3 scaling segment is inserted before the 1/2 segment, as illustrated in Fig. 5.4. 84 5 Scaling Analysis of Polymer Dynamics
9. 9. 5.3 Long Chains When a long chain diffuses within its bulk melt phase, it remains a coil-like shape containing many other interpenetrated chains. The other chains are not allowed to diffuse together with this chain; rather, they block local vertical diffusion along the contour length of this chain due to the volume exclusion effect, which is often called the entanglement effect. Such entanglements force the chain to diffuse mostly along its contour length, behaving like a snake. Edwards ﬁrst proposed the tube model (Edwards 1967). He regarded such entanglements around the primitive path of the long chain to form an effectively dynamic network, and to trap the long chain in a tube, as demonstrated in Fig. 5.5. De Gennes later-on proposed the reptation model (De Gennes 1971). He assumed the tube diameter a (about 10 nm) and n/ne blobs, each with the size of a, forming the tube length Z ~ an/ne, where ne is the critical chain length for the effect of chain entanglement. a2 \$ neb2 (5.44) The characteristic time for the chain to diffuse out of the tube is tt ¼ Z2 Dt (5.45) Log10[r(t)-r(0)]2 Log10t 1 1/2 1 τ0 τR b2 nb 2 C -1/4 τξ 2/3 g 6/5 b2 Zimm Rouse Fig. 5.4 Double logarithmic plot of the mean-square displacements of monomers versus the time for the scaling laws for a short chain in semi- dilute solutions. The Zimm chains are slightly faster than the Rouse chains due to their less frictional barrier in the non-draining mode Fig. 5.5 Illustration of the tube model for a long chain diffusing in the bulk phase 5.3 Long Chains 85
10. 10. Imagining that the frictional barrier for the motion of each blob is integrated into that for the motion of the whole chain, thus zt ¼ z n ne (5.46) From the Einstein relationship D ¼ kT/z, one obtains Dt ¼ kT zt ¼ kTne zn ¼ Dne n (5.47) Therefore, the characteristic time for the reptation model becomes tt \$ n2 Dt \$ n3 (5.48) The reptation time exhibits stronger chain-length dependence than the Rouse time (tR ~ n2 ). Accordingly, the diffusion coefﬁcient is Drep ¼ R2 tt ¼ nb2 tt \$ nÀ2 (5.49) The diffusion coefﬁcient for the reptation chain shows weaker chain-length dependence than that for the Rouse chain (DR ~ nÀ1 ). Both (5.48) and (5.49) imply that the tube makes an additional conﬁnement to the self-diffusion of the polymer chains. Therefore, the long chains diffuse slower, and the diffusion coefﬁcient becomes more sensitive to the chain length. The primitive path of the long chain reveals the characteristic feature of the reptation model for the diffusion of an ideal chain. Since tR tt, polymer chains perform the Rouse-chain motions along the tube before they diffuse out of the tube. Therefore, within the time window between the relaxation time of critically entangled chain te and the relaxation time of the reptation tube tt, monomers diffuse through a certain length of the tube. Meanwhile, the tube itself can be regarded as a contour of an ideal chain, and the tube length is proportional to the mean-square end-to-end distance, which corresponds to the total mean-square displacement of each monomer. Note that the tube length is the sliding diffusion distance of the Rouse chain, then ½rðtÞ À rð0Þ2 rep \$ tube length ¼ rðtÞ À rð0ÞR \$ ½rðtÞ À rð0Þ2 1=2 R (5.50) In other words, within the time period from te to tt, the polymer chain diffuses along the tube with the Rouse mode. Owning to the tube conﬁnement, the scaling exponent of the original Rouse chain has been reduced into half. Therefore, the 86 5 Scaling Analysis of Polymer Dynamics
11. 11. reptation chain diffuses even slower than the Rouse chain. The overall scaling relationships of the chain dynamics for the reptation chain can be summarized below, as also demonstrated in Fig. 5.6. [r(t)-r(0)]2 rep ~ t, if t t0; (within the scale of b2 ) ~t1/2 , if t0 t te; (within the scale of a2 ) ~t1/4 , if te t tR; (within the scale of n1/2 ab) ~t1/2 , if tR t tt; (within the scale of nb2 ) ~t, if tt t. Similar to the scaling analysis for the short chains in concentrated solutions, we can assume the screening length of hydrodynamic interactions for the long chains, corresponding to the screening length of the volume repulsive interactions, as xh % x (5.51) Applying the blob model, one can obtain x \$ g3=5 \$ CÀ3=4 (5.52) At the motion length scale smaller than xh, the Zimm-chain model is valid. In contrast, at the motion length scale above xh, there occur two different scenarios: the Rouse-chain model is applicable at the scale smaller than the critical entangle- ment length ne; and the reptation-chain model is applicable at the scale larger than ne. The results are similar with the semi-dilute solutions of short chains, withtx between t0 and te, i.e. inserting 2/3 scaling exponent before 1/2 scaling exponent. In the following, we discuss two examples to demonstrate how the results of scaling analysis facilitate our better understanding to the deformation and ﬂow behaviors of polymer chains. A very small stress s working on the polymer melt will reveal the elastic response of the ﬂuid, and the strain eðtÞ ¼ s Á JðtÞ (5.53) τe Log10[r(t)-r(0)]2 Log10t 1 1/2 1 τ0 τt b 2 nb 2 τR 1/2 n 1/2 ab 1/4 a 2 Rouse chain Reptation chain Fig. 5.6 Double logarithmic plot of the mean-square displacements of monomers versus the time for the scaling law of a long chain in the bulk polymer phase. Reptation chains are slower (half-down indexes) than Rouse chains due to the tube conﬁnement 5.3 Long Chains 87
12. 12. where J(t) is called the time-dependent creep compliance. When t tt, polymer chains are trapped in an elastic network of entanglements, and the compliance shows a plateau as the time increases, which is characteristic for the long-chain melt. JðtÞ ! J0 (5.54) where J0 is the steady-state compliance, as demonstrated in Fig. 5.7. The corresponding plateau modulus, E0 ¼ 1 J0 (5.55) and the corresponding equation of state for the transient rubber state is E0 ¼ ckT Ne (5.56) where c ¼ 1/a3 , and a is the size of the monomers. The critical molecular weight of polystyrene 1.13 Â 104 g/mol corresponds to a plateau modulus of 2.24 Â 105 Pa, in agreement with the experimental observations, 2 Â 105 Pa (Sperling 2006). When t tt, the chain eventually “reptates” out of the tube. Under the stress, polymer melt can perform the steady-state ﬂow with a permanent deformation, thus JðtÞ ¼ J0 t tt (5.57) From a Newtonian ﬂuid s ¼ deðtÞ dt (5.58) Then we can obtain the melt viscosity ¼ dt dJðtÞ ¼ tt J0 ¼ E0tt (5.59) Fig. 5.7 Illustration of the rubber plateau for the creep compliance within the time scale shorter than the characteristic time of the reptation chain in the melt phase at a given temperature 88 5 Scaling Analysis of Polymer Dynamics
13. 13. For the short chains in the melt phase, the whole chain could not relax within the time scale of the Rouse time, but rather forms a dynamic network to display an elastic response to the external stress. According to (5.56), we have E0 ¼ ckT n (5.60) Therefore, R \$ E0tR \$ 1 n Á n2 ¼ n (5.61) For the reptation model, E0 ¼ ckT ne (5.62) Therefore, rep \$ E0tt \$ n3 (5.63) The experimental observations on the zero-shear melt viscosity reveal that, for the chain length below ne (more exactly 2ne), the scaling relation indeed follows the prediction of the Rouse-chain model, while above ne, it shows an index of 3.4, quite close to the 3.0 predicted by the reptation-chain model, as demonstrated in Fig. 5.8. Doi proposed to consider the contour length ﬂuctuations (CLF), which theoretically corrects the scaling exponent to 3.5 (Doi 1983). The molecular-weight index of the self-diffusioncoefﬁcient can be further corrected into À2.25, close to the experimental observation À2.3 (Frischknecht and Milner 2000). Recently, Liu et al. reported that the deviation of the exponent from 3.0 might be attributed to cooperative motion of multiple chains (Liu et al. 2006). For ﬂexible chains, experimental studies found that when the molecular weight is higher than a critical value Mr, the scaling exponent returns to 3.0 (Colby et al. 1987). The tube length is sufﬁciently long so that its length ﬂuctuations might not be important anymore. Presently, the inﬂuences of polydispersity and chain branching on the dynamics of polymers have been analyzed theoretically. The disentanglement along the reptation of a long chain is accelerated by the surrounding short chains due to the Fig. 5.8 Illustration of the scaling relationship between the zero-shear viscosity and the molecular weight. Here ne should be more precise as 2ne 5.3 Long Chains 89
14. 14. faster diffusion of the latter. Hence, the local constraint on the tube shape conﬁning the long chain is released, which is called thermal constraint release (TCR). Therefore, in a polydisperse system, the diffusion coefﬁcients of long-chain fractions are highly related to the short-chain fractions, and the polydispersity affects the chain motion of polymers (Graessley 1982). After the thermal constraint release, the distance between two neighboring entanglement points along the chain is increased. Therefore, the corresponding radius of the local tube is enlarged (Milner and McLeish 1997). Such a situation is often called dynamic tube dilation (DTD). The DTD model can be applied to the chain dynamics of long-chain- branching polymers like star-shape polymers. Since the branching point diffuses relatively slowly, the arm retraction (AR) can be further considered on the basis of the Rouse-chain model. The characteristic relaxation time of long-chain branches is extremely long, and the viscosity does not rely on the number of arms, but rather, exponentially on the length of arms. Once the whole polymer is stretched, its retraction becomes extremely difﬁcult, which is a phenomenon known as extensional-hardening (McLeish 2002). The details of theoretical treatments can be found from the literature mentioned above. More challenges still remain, regarding the inﬂuence of chain rigidity, nano-conﬁnement, heterogeneous phases and charge interactions on the chain dynamics, which are prevailing in bio-macromolecules and playing important roles in various living processes. Question Sets 1. Why do we say that the Rouse-chain model rests on the ideal-chain model? 2. Why does the Zimm chain run faster than the Rouse chain? 3. Why can the reptation-chain model describe the Brownian motions of long- chain polymers? 4. Why do polymers have a rubber plateau between the glass state and the liquid state? 5. What are the characteristics of branched-chain motions? References Colby R, Fetters LJ, Graessley WW (1987) Melt viscosity - molecular weight relationship for linear polymers. Macromolecules 20:2226–2237 De Gennes PG (1971) Reptation of a polymer chain in a presence of ﬁxed obstacles. J Chem Phys 55:572–579 Des Cloizeaux J, Jannink G (1990) Polymers in solution: their modelling and structure. Oxford University Press, Oxford Doi M (1983) Explanation for the 3.4 power-law for viscosity of polymeric liquids on the basis of the tube model. J Polym Sci Polym Phys 21:667–684 Edwards SF (1967) The statistical mechanics of polymerized material. Proc Phys Soc 92:9–13 Einstein A (1905) Investigations on the theory of the Brownian movement. Ann Phys (Leipzig) 17:549–560 Einstein A (1911) Eine neue Bestimmung der Molekuldimensionen. Ann Phys (Leipzig) 34:591–592 90 5 Scaling Analysis of Polymer Dynamics
15. 15. Fox TG, Flory PJ (1948) Viscosity-molecular weight and viscosity- temperature relationships for polystyrene and polyisobutylene. J Am Chem Soc 70:2384–2395 Frischknecht AL, Milner ST (2000) Diffusion with contour length ﬂuctuations in linear polymer melts. Macromolecules 33:5273–5277 Graessley WW (1982) Entangled linear, branched and network polymer systems-molecular theories. Adv Polym Sci 47:67–117 Houwink R (1940) Relation between the polymerization degree determined by osmotic and viscometric methods. J Prakt Chem 157:15–18 Kirkwood JG, Riseman J (1948) The intrinsic viscosities and diffusion constants of ﬂexible macromolecules in solution. J Chem Phys 16:565–573 Kuhn W (1934) Fadenformiger Molekule in Losungen. Kolloid-Z 68:2–15 Liu CY, Keunings R, Bailly C (2006) Do deviations from reptation scaling of entangled polymer melts result from single or many chain effects? Phys Rev Lett 97:246001 Mark H (1938) U¨ ber die entstehung und eigenschaften hochpolymerer festko¨rper. In: Sa¨nger R (ed) Der feste Ko¨rper. Hirzel, Leipzig, pp 65–104 McLeish TCB (2002) Tube theory of entangled polymer dynamics. Adv Phys 51:1379–1527 Milner ST, McLeish TCB (1997) Parameter-free theory for stress relaxation in star polymer melts. Macromolecules 30:2159–2166 Nyquist H (1928) Thermal agitation of electric charge in conductors. Phys Rev 32:110–113 Rouse PE (1953) A theory of the linear viscoelastic properties of dilute solution of coiling polymers. J Chem Phys 21:1273–1280 Sperling LH (2006) Introduction to physical polymer science, 4th edn. Wiley, New York, p 526 Staudinger H, Nodzu R (1930) U¨ ber hochpolymere Verbindungen, 36. Mitteil: Viscosita¨ts- Untersuchungen an Parafﬁn-Lo¨sungen. Berichte der Deutschen Chemischen Gesellschaft 63:721–724 Stokes GG (1851) On the effect of the internal friction of ﬂuids on the motion of pendulums. Trans Camb Phil Soc 9(Pt. II):8–106 Zimm BH (1956) Dynamics of polymer molecules in dilute solution: viscoelasticity. J Chem Phys 24:269–278 References 91